Nuclear Magnetic Resonance and ElectronParamagnetic Resonance as Analytical Tools ToInvestigate Structural Features of ArchaeologicalLeathers
Michel Bardet,*, Guillaume Gerbaud, Laurent Le Pape,, Sabine Hediger,,| Quoc-Khoi Tran,
and Nebia Boumlil
Laboratoire de Resonances Magnetiques, INAC, SCIB, Laboratoire de Chimie et Biologie des Metaux, iRTSV,ARC-Nucleart, CEA, F-38054 Grenoble, France, and Laboratoire de Chimie (UMR 5182 CNRS/ENS), Laboratoire deRecherche Conventionne du CEA (DSM-04-32), Ecole Normale Superieure de Lyon, F-69364, France
Archaeological waterlogged leathers dated from the 13thto 17th century have been analyzed using carbon-13 high-resolution solid-state nuclear magnetic resonance (NMR)and electron paramagnetic resonance (EPR). The NMRand EPR spectra have been compared to modern vegetable-tanned leathers and crude hide. Both techniques allowedus to fully characterize the samples and better understandthe changes occurring during aging in water environment.The main features of the archaeological leathers are thehigh contents in iron and the absence of residual vegetabletannins. Traces of lubricants could not be detected either.The accumulation of iron oxides may have played a rolein the conservation of the archaeological objects andexplain the surprising good conservation state of theleather samples as was observed in the NMR spectra. Theabsence of tannins and lubricants in the studied archaeo-logical samples is also discussed. It may be a conse-quence of aging in water-rich environment. The analysisstrategy described in this paper can be systematicallyapplied to characterize archaeological or historical leathersamples.
Leather production is certainly one of the most ancientindustrial activities still in operation.1 The chemistry involved inleather making and its deterioration over time has been animportant field of study for a long time. As a matter of fact, bothhistorical and archaeological leathers represent an important partof the cultural patrimony all over the world that must betransferred from generation to generation. The preservation ofartifacts made entirely or partially of leather is very challenging,as it is a particularly difficult material to conserve. This difficultyarises undoubtedly from the nature of the raw hide itself and fromthe different processes involved in its transformation into leather.
Macroscopic properties of leather, making it suitable for artifactmanufacturing, rely mainly on the applied tanning processes.These latter involve either organic compounds, such as naturaltannins extracted from different woody plants, or mineral tannins,such as different varieties of native alum mainly used before the18th century. They are all known to create molecular covalent orvan der Waals interactions with the collagen moiety of skins. Oneof the targets of the tanning process is to favor molecularinteractions inside the entire volume of the starting hide. Lubri-cants, such as oils or fats, can be also introduced into the leatherdirectly as a tanning agent or at the end of the tanning process inorder to increase and maintain its flexibility and softness proper-ties. Lubricants also reduce water absorption. At room temperaturelubricants are either liquids or soft solids, and even after theirincorporation in the leather, they generally keep a high degreeof molecular mobility.
In this article we illustrate the potential of solid-state 13C NMRspectroscopy2-5 to investigate the structural properties of ar-chaeological leathers and to follow their changes under aging.Surprisingly, up to now only a very few high-resolution solid-stateNMR studies have been devoted to historical or archaeologicalleathers compared to other bio-organic compounds such aslignocellulosic materials,6-11 although the analysis strategy is verysimilar in both cases. Only a few NMR studies are reported onhistorical parchments.12,13 In this work, electron paramagneticresonance (EPR) was used as well to gain valuable informationon the presence and the role of iron and manganese oxides in
* To whom correspondence should be addressed. Phone: 33 04 38 78 57 75.Fax: 33 04 38 78 50 90. E-mail: email@example.com.
Laboratoire de Resonances Magnetiques, INAC, SCIB, CEA. Laboratoire de Chimie et Biologie des Metaux, iRTSV, CEA. ARC-Nucleart, CEA.| Ecole Normale Superieure de Lyon.
(1) Kite, M.; Thomson, R. Conservation of Leather and Related Material;Butterworth & Co.: Oxford, U.K., 2006.
(2) Smit, Z.; Petru, S.; Grime, G.; Vidmar, T.; Budnar, M.; Zorko, B.; Ravnikar,M. Nucl. Instrum. Methods Phys. Res., Sect. B 1998, 140, 209216.
(3) Simunkova, E.; Skvaril, L. Sb. Vys. Sk. Chem.-Technol. Praze, S: Polym.sChem.,Vlastnosti Zprac. 1985, S13, 6368.
(4) Spiess, H. W. Chem. Rev. 1991, 91, 13211338.(5) Spiess, H. W. Annu. Rev. Mater. Sci. 1991, 21, 131158.(6) Ghisalberti, E. L.; Godfrey, I. M. Stud. Conserv. 1998, 43, 215230.(7) Lambert, J. B.; Shawl, C. E.; Stearns, J. A. Chem. Soc. Rev. 2000, 29, 175
182.(8) Gill, A. M.; Neto, C. P. Annu. Rep. NMR Spectrosc. 1999, 37, 7577.(9) Bardet, M.; Foray, M. F.; Tran, Q. K. Anal. Chem. 2002, 74, 43864390.
(10) Bardet, M.; Foray, M. F.; Maron, S.; Goncalves, P.; Tran, Q. K. Carbohydr.Polym. 2004, 57, 419424.
(11) Pournou, A. Archaeometry 2008, 50, 129141.(12) Odlyha, M.; Cohen, N. S.; Foster, G. M.; Aliev, A.; Verdonck, E.; Grandy,
D. J. Therm. Anal. Calorim. 2003, 71, 939950.(13) Aliev, A. E. Biopolymers 2005, 77, 230245.
Anal. Chem. 2009, 81, 15051511
10.1021/ac802052a CCC: $40.75 2009 American Chemical Society 1505Analytical Chemistry, Vol. 81, No. 4, February 15, 2009Published on Web 01/21/2009
the archaeological samples. It is worth noting that in archaeologi-cal sciences EPR has been used several times to study inorganicmaterials14,15 but never, as far as we know, for organic materialssuch as woods and leathers.
High-resolution solid-state NMR leads to structural informationon organic compounds through qualitative analyses, quantitativemeasurements, and molecular dynamic studies.16 It can readilybe applied to investigate tanning and post-tanning treatments, aswell as aging of leathers under different external conditions. Inthis work we focus on the qualitative approach of solid-state NMRusing mainly two basic experiments. On the one hand, thecommonly used CP-MAS experiment, which combines proton-to-carbon cross-polarization transfer (CP) and magic-angle samplespinning (MAS), allows the carbons of rigid domains to beselectively observed. On the other hand, carbons of mobiledomains can be selectively observed through direct 13C observa-tion by single-pulse excitation (SP) and high-power decouplingapplied during signal acquisition. To obtain high-resolutionspectra, the SP experiment is also combined with MAS, andthe full experiment is denoted the SP-MAS experiment. Inmodern leather, collagen and tannin moieties are typical rigidpolymers on the NMR point of view and appear in CP-MASspectra, whereas all lubricants used to soften the leather areselectively observed with the SP-MAS experiment. As aconsequence carbons belonging to different domains of mobil-ity can be edited in separated spectra by combining CP-MASand SP-MAS experiments.17 As we have already shown on otherorganic materials, typical solution NMR experiments such asDEPT (distortionless enhancement by polarization transfer) canbe as well directly applied when molecular mobility is highenough for MAS alone to completely average to zero thereduced proton-proton dipolar interactions and the magneticsusceptibility tensor. DEPT allows specific editing of subspectraof CH, CH2, and CH3 carbons.18
The waterlogged leather samples studied in this work werecollected from an excavation in Lyon, France during the buildingof a car parking at the St-Georges area. They were clearlyidentified to soles of shoes and were dated from the 13th to 18thcentury. They constitute a valuable set of well-identified archaeo-logical samples that have allowed us to illustrate the interest inarchaeological sciences of solid-state NMR and EPR spec-troscopies. Their structural features, obtained from NMR and EPR,are compared here to those of modern leathers.
EXPERIMENTAL SECTIONSample Preparation. The waterlogged leather samples, dated
from the 13th to 18th century, were collected during the years1996-1998 from an excavation in Lyon, France at the St-Georgesarea. The samples were washed with fresh water to remove any
mud particles and kept at 5 C in water with antiseptics to preventbiological degradation. Before analyses, they were washed againand dried for 1 week inside a fume hood under strong ventilationuntil they reached constant weights. The amount of watercontained in the wet sample was measured from these experi-ments. The commercially available crude tannins and the modernleather samples tanned with vegetable tannins were kindlyprovided by Guy Lumia at CEA-Marcoule, France. Among them,a first sample was treated with tannins extracted from quebrachoand a second one with oak leaf tannin. They are denoted in thefollowing quebracho leather and oak leather, respectively. Athird sample, denoted moroccan leather, whose vegetable tanninprocess is not known, was provided from a small-scale leatherproduction. Crude collagen was purchased from Sigma. Thecorium-layer sample was directly prepared at the laboratory fromthe salted hide of a 17 month old beef obtained at theslaughterhouse.
NMR Experiments. For each sample, 300-400 mg of driedmaterial was cut in a small cube of 2-3 mm edge and filled in 7mm diameter (340 L) cylindrical double-bearing rotors made ofzirconia. The rotors were closed with Kel-F end caps. All high-resolution solid-state 13C NMR spectra were recorded at roomtemperature on a Bruker Avance DSX 200 spectrometeroperating at a proton frequency of 200.13 MHz (carbonf